A comparative experimental study on the cross-plane thermal conductivities of nano-constructed Sb2Te3/(Cu, Ag, Au, Pt) thermoelectric multilayer thin films
- 841 Downloads
Thermoelectric multilayer thin films used in nanoscale energy conversion have been receiving increasing attention in both academic research and industrial applications. Thermal transport across multilayer interface plays a key role in improving thermoelectric conversion efficiency. In this study, the cross-plane thermal conductivities of nano-constructed Sb2Te3/(Cu, Ag, Au, Pt) thermoelectric multilayer thin films have been measured using time-domain thermoreflectance method. The interface morphology features of multilayer thin film samples were characterized by using scanning and transmission electron microscopes. The effects of interface microstructure on the cross-plane thermal conductivities of the multilayer thin films have been extensively examined and the thermal transfer mechanism has been explored. The results indicated that electron–phonon coupling occurred at the semiconductor/metal interface that strongly affected the cross-plane thermal conductivity. By appropriately optimizing the period thickness of the metal layer, the cross-plane thermal conductivity can be effectively reduced, thereby improving the thermoelectric conversion efficiency. This work presents both experimental and theoretical understanding of the thermal transport properties of Sb2Te3/metal multilayer thin film junctions with important implications for exploring a novel approach to improving the thermoelectric conversion efficiency.
KeywordsThermoelectric thin films Cross-plane thermal conductivity Time-domain thermoreflectance (TDTR) Electron–phonon coupling
With the ever increasing of energy demanded, to develop sustainable energy sources strategy becomes more and more concerned in recent years, Thermoelectric technology, harvesting electric power from heat, is a promising environmentally friendly means of energy conversion. The thermoelectric technology has an inherent advantage to harvest widely distributed waste heat, and also proved as an alternative route to convert solar energy into electric power economically . In addition, the thermoelectric system also has other unique advantages such as small size, high reliability, no pollutants, and feasibility over a wide temperature range . However, the current conversion efficiency of thermoelectricity is much less than that of equivalent mechanical systems. For this reason, thermoelectricity has been long limited to engineering or commercial application. Therefore, improving the conversion efficiency of thermoelectric devices is one of the most important challenges in the fields of energy harvesting.
The thermoelectric energy conversion efficiency is determined by the dimensionless figure of merit ZT, where Z is a measure of a material’s thermoelectric properties and T is absolute temperature. The materials coefficient Z is expressed in term of Seebeck coefficient S, electrical conductivity σ and thermal conductivity κ, yielding equation Z = S2·σ/κ. To maximize the ZT value of thermoelectric device, a large Seebeck coefficient, high electrical conductivity, and low thermal conductivity are therefore most expected [3, 4]. In order to improve the thermoelectric efficiency, various approaches to enhancing ZT have been proposed and developed.
In the early 1990s, Hicks and Dresselhaus pointed out that low-dimensional thermoelectric materials exhibit a significant enhancement in ZT value [5, 6, 7]. The enhancement mechanism can be attributed to two facts, one involving the increase in the power factor (S2·σ) by quantum confinement effects, which enhanced the density of states near the Fermi energy [8, 9, 10], and the other involving the reduction in thermal conductivity by tailoring the nanostructure . The idea of selectively modifying thermoelectric material properties using lower-dimensional nanostructures has been successful developed in the subsequent years [12, 13].
Nanostructured thermoelectric materials offer a new way of improving thermoelectric conversion performance by tailoring electron and phonon transport properties [14, 15]. Two-dimensional (2D) multilayer thin films or superlattice structures can significantly enhance the ZT values of thermoelectric materials since electrons are confined to move in two dimensions and phonons can be effectively scattered by the high density of interfaces, which results in a decrease in the lattice thermal conductivity [16, 17]. Abundant experimental and theoretical studies have indicated that nanoscale multilayer thin films or superlattice have lower thermal conductivities than their conventional bulk materials as a result of size and interface effects [18, 19, 20, 21]. Of special note, the traditional phenomenological heat transfer equations are not applicable at the nanoscale; the investigation or analysis of the thermal transport mechanism in the multilayer thin film system belongs to the catalog of micro/nanoscale heat transfer . Scientific understanding of the thermal transport occurring in the nanoscale multilayer thin structures is highly necessary and exigent [23, 24]. Recently, the thermal conductivities of periodic thin film structures have been extensively investigated by Hopkins et al. [25, 26, 27, 28, 29], Xiao et al. , and Cahill et al. . The results indicated that the transport of electrons and phonons in nanoscale multilayer thermoelectric thin films is mainly affected by the presence of interfaces and defects, and that the minimum thermal conductivity of a multilayer thin film or superlattice can be realized by optimizing its nanostructure [32, 33, 34]. In a series of papers, Chen et al. reported on their investigations of the ballistic-phonon transport occurring in the cross-plane direction of superlattices [34, 35, 36] that revealed the heat conduction mechanisms in the periodic thin-film structures. Hopkins et al. studied the effects of interfacial properties (roughness, disorder, dislocations, and bonding) on the cross-plane thermal conductivity of a multilayer thin film structure [25, 26, 29], and indicated that the cross-plane thermal conductivity can be further reduced by controlling the interface morphology . However, the interfacial properties of multilayer thin films are closely related to the pair of the composed materials. Several studies indicated that ultralow thermal conductivities of the multilayers can be realized by choosing the pair of thermoelectric materials properly [37, 38, 39].
In this investigation, the cross-plane thermal conductivities of nanostructured Sb2Te3/(Cu, Ag, Au, Pt) thermoelectric multilayer thin films have been experimentally studied. The thermal transfer mechanism (i.e., size and interface effects) has been explored in combination with experimental measurements and modal analyses. The total effects of multilayer nanostructure on the cross-plane thermal conductivity of the thermoelectric thin film has been evaluated according to the obtained results, with the ultimate goal being to provide useful guidance and help for the practical thermoelectric engineering applications.
2 Sample preparation
Low-dimension thermoelectric multilayer thin film preparation processes are generally categorized into two groups: physical and chemical processes, each having its own advantages and disadvantages. The choice of method mainly depends on the cost of processing or material properties. In general, physical methods include magnetron sputtering, electron beam physical vapor deposition, and molecular beam epitaxy, which inherently need a high-vacuum environment. The chemical processes include electrochemical deposition and metal-organic chemical vapor deposition, as well as other synthesis methods. These methods are more suitable for large-area deposition. In most cases, thermoelectric multilayer thin films are fabricated by physical methods depending on their properties and the applications. Among the various physical approaches, magnetron sputtering is commonly used. Magnetron sputtering has advantages compared to most thermal evaporation techniques: (i) the composition of the sputtered material is the same as that of the target, resulting in higher quality of the samples; (ii) the evaporation conditions are stable and easily controlled by plasma current; (iii) the heat load on the chamber walls is far smaller, reducing outgassing and subsequent impurity incorporation by reactive particles .
In this experiment, the bilayer thin films were prepared by alternate sputtering onto a Si substrate in a high-vacuum magnetron sputtering system (Denton, explorer-14, USA) at room temperature. The independent metal targets have high purity (99.999%). Before the process, the Si substrate was soaked in B.O.E solution (HF: NH4F = 1:6) for 5–10 min to chemically etch off the surface oxide layer, and then, was ultrasonically cleaned in acetone and ethanol solutions for 10 min. After drying with high purity nitrogen gas, the substrate was transferred into a sputtering chamber and mounted on the holder. The distance between the targets and substrate was about 200 mm. The sputtering pressure was set at 3 mTorr and the substrate pressure was controlled at 2 × 10−7 Torr. A calibrated quartz crystal monitor was used to measure the deposition rate. During the deposition, the power was applied in radio frequency (RF) mode for Sb2Te3 and direct current (DC) mode for Au, Ag, Cu, and Pt. In addition, the substrate was rotated at the speed of 20 rpm to ensure deposition uniformity. The total thickness of the thermoelectric multilayer thin film was about 300 nm.
3 Multilayer structure characterization and analysis
The multilayer thin structure is strongly correlated to its thermal and physical properties. Particularly, the size and interface effects on the cross-plane thermal conductivity need to be further investigated. In order to explore comprehensively the interface effects on the thermal transport properties of the multilayer thin film, the cross-section morphology was observed by scanning electronic microscopy (SEM) and using a transmission electron microscope (TEM).
Figure 3 shows the interface roughness between the Sb2Te3 and metal period layers. The interface roughness can affect phonon reflection and transmission at the interface; therefore, it can have a significant effect on the cross-plane thermal conductivity of the multilayer thin film. On the other hand, atomic scale interface roughness does not cause a significant reduction in electron mobility, since the typical electron coherence length in semiconductors is much longer than that of phonons, and it can be reflected specularly . Hence, by constructing nanoscale Sb2Te3/metal multilayer thin film properly, it can reduce the cross-plane thermal conductivity without deterioration in electron transfer, thus improving the thermoelectric conversion efficiency. In practical engineering, the interface roughness correlated with certain sputtering parameters, such as Ar pressure, bias voltage, sputtering power and substrate temperature. It can be effective controlled by adjusted the bias power during fabrication.
The atomic scale lattice structures of Sb2Te3 and Au at the interface can be clearly observed in Fig. 4. It shows the lattice dislocations at the Sb2Te3-metal layer interface. In fact, the lattice dislocations between the Sb2Te3 and metal in the multilayer structure can lead to a remarkable difference in the thermal and physical properties of the thin film systems. In addition, it probably had an influence on phonon transport. The lattice-dislocations interface with defects and mixing may affect the phonon transmission and significantly change the cross-plane thermal conductivity. To some extent, lattice dislocations or misfits at the multilayer interface can enhance phonon scattering, thereby reducing the thermal conductivity of the lattice . Interfacial dislocations can enhance phonon or electron scattering, thereby reducing the lattice or electron thermal conductivity.
4 Experimental procedure
In this experiment, the cross-plane thermal conductivities of nano-constructed Sb2Te3/(Cu, Ag, Au, Pt) thermoelectric multilayer thin film samples were measured by time-domain thermoreflectance (TDTR) method. The measurements were carried out in the National Laboratory of Solid State Microstructures of Nanjing University. Currently, TDTR was developed as a reliable and convenient non-contact technique for determining the thermal conductivities of nanostructured materials. Before the TDTR measurements, a compact Al film with a thickness of 80 nm was deposited on the thin film surface to serve as an optical transducer. The output of a Ti: sapphire oscillator laser was split into a pump beam and a probe beam with a relative delay time of 0–4000 ps. The modulated pump beam heated the Al surface periodically, creating a temperature fluctuation at 9.8 MHz. This fluctuation was then detected by the probe beam due to the linear temperature dependence of optical reflectivity on the Al surface and was recorded by a lock-in amplifier. The cross-plane thermal conductivity was obtained by fitting the measurement signals to a diffusive thermal model. In this experiment, every measurement was repeated three times, and the average value was obtained. In addition, we strictly checked the experimental errors before and after each measurement. More details about the measurement, data analysis, and modeling can be found elsewhere [42, 43, 44]. In addition, to verify the measurement data, we also employed the standard differential 3ω method to measure and compare the obtained results with those obtained from the TDTR method.
5 Results and discussion
5.1 Cross-plane thermal conductivities of Sb2Te3/(Cu, Ag, Au, Pt)multilayer thin films with various period thickness
It can be seen from Fig. 5 that the cross-plane thermal conductivities of Sb2Te3/(Cu, Ag, Au, Pt) multilayer thin films increase with the period thickness in a specific range (larger than 200 Å). The reason can be attributed to two aspects, one involving the increased proportion of the metal composition, and the other involving the reduction in the density of the interface. However, for the same period thickness, it can be found from Fig. 5 that the cross-plane thermal conductivity of Sb2Te3/Ag exhibits the minimum value compared to those of the Sb2Te3/(Cu, Au, Pt) thermoelectric multilayer thin films. In contrast, Sb2Te3/Pt reveals a high cross-plane thermal conductivity in all the samples investigated. There are two possible reasons responsible for the deviation of thermal conductivity of Sb2Te3/Ag and Sb2Te3/Pt multilayer film. One is the interface condition; it can be seen from the Fig. 1 that Sb2Te3/Pt film has good film forming characteristics than Sb2Te3/Ag film. The larger interface roughness of Sb2Te3/Ag multilayer thin film has a significant effect on phonon scattering, thereby reducing the thermal conductivity. Another reason is electron–phonon coupling occurred at interface of various materials pairs.
It can be seen from Fig. 6 that the modeling results agree well with the measured data. The results indicate that the electron–phonon coupling mechanism plays an important role in determining the interfacial thermal resistance and that the effective thermal conductivities are affected by the nonequilibrium process between the electrons and phonons on the metal side. Based on analysis of the model, it can be found that the coupling factor G at the Sb2Te3-metal interface is in the range 1016–1017 W/m3K. Therefore, by choosing a proper period thickness of the metal layer, which changes the coupling length appropriately, the thermal conductivity of the metal-semiconductor multilayer thin film could be further reduced.
5.2 Cross-plane thermal conductivities of Sb2Te3/Au multilayer thin films at various temperatures
For simplified calculations, a linear Debye approximation of the phonon dispersion relation has been employed. After obtaining the interfacial thermal conductance, we could model the total thermal resistance; finally, the effective thermal conductivity could be simply evaluated according to ke = (d1 + d2)/2(R1→2). The obtained results were compared with the experimental data, as shown in Fig. 7. Of special note, a big assumption has been made in the present model in that the material structure is perfectly crystalline. However, the Sb2Te3/Ag multilayer thin film is polycrystalline or amorphous structure. Here, there are fairly large discrepancies between the experimental data and the predicted model results, even though the model provides better understanding of heat transport for the multilayer thin films at various temperatures.
In this study, the cross-plane thermal conductivities of nanostructured Sb2Te3/(Cu, Ag, Au, Pt) thermoelectric multilayer thin film systems were investigated. The effects of interface microstructure on the thermal conductivity of the multilayer thin film were examined. In addition, the temperature profile was also investigated. The experimental results indicated that nanometer multilayer interface microstructures have a significant effect on the cross-plane thermal conductivity. The nanometer interface microstructure could influence phonon scattering process. In addition, the experimental and model results suggested that, for Sb2Te3/metal (Cu, Ag, Au, and Pt) thermoelectric multilayer thin films, the electron–phonon coupling that occurred at the interface also influenced the cross-plane thermal conductivity of multilayer thin film. By optimizing the material system properly, the cross-plane thermal conductivities of thermoelectric multilayer thin films can be further reduced without deteriorating the electron transfer properties. However, the correlation between microstructure and thermal conductivity still needs to be explored. More important, the thermal transport mechanisms at the atomic scale need to be revealed. In addition, experimental study indicated that the cross-plane thermal conductivity of semiconductor/metal thermoelectric multilayer thin film increased with period thickness of the metal layer, which suggested that electron thermal conductivity contributed a certain proportion to total thermal conductivity. For the Sb2Te3/metal (Cu, Ag, Au, Pt) multilayer thin films, interface effects and electron–phonon coupling effects dominated its thermal transport properties. In conclusion, cross-plane thermal conductivity reduction by engineering interface conditions may offer a promising route to improve thermoelectric conversion efficiency.
GY and JP contributed equally to this work; XF and YW contributed to fabrication. XJY and MHL contributed to experiments. ZW and EM contributed to manuscript preparation. ZH directed entire research at Shanghai Jiao Tong University and contributed to the manuscript preparation. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
This research was supported by National Natural Science Foundation of China (Grant No: 5177060654), China Postdoctoral Science Foundation (Grant No: 2017M611560). Ministry of Science and Technology of China (2009DFB60160), Yunnan Hu Zhiyu Expert Workstation ( 5). We also would like to thank the Center for Advanced Electronic Materials and Devices (AEMD) of Shanghai Jiao Tong University and Instrumental Analysis Center and the startup fund of Shanghai Jiao Tong University.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
- 2.X. Zhang, L.-D. Zhao, J. Metr. 1, 92 (2015)Google Scholar
- 3.G. Slack, CRC handbook of thermoelectrics (CRC Press, Boca Raton, 1995)Google Scholar
- 13.G. Pennelli, Beilstein. J. Nanotechnol. 5, 1268 (2014)Google Scholar
- 22.Z.M. Zhang, Nano/microscale heat transfer (McGraw-Hill, New York, 2007)Google Scholar
- 25.P.E. Hopkins, L.M. Phinney, in 14th International Heat Transfer Conference (2010)Google Scholar
- 29.P.E. Hopkins, ISRN Mechanical Engineering 2013, 1 (2013)Google Scholar
- 49.G.J. V, M. B, in Semiconductor Thermal Measurement and Management Symposium (SEMI-THERM), 27th Annual IEEE (2011)Google Scholar
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.